poly(vinyl chloride)/tio2 nanocomposite resin via the ... ?· poly(vinyl chloride)/tio 2...
Post on 15-Aug-2019
Embed Size (px)
Poly(vinyl chloride)/TiO2 nanocomposite resin via the synthesis of TiO2 nanoparticles in vinyl chloride followed by in situ suspension polymerization
H. Yoo* and S.-Y. Kwak**
Department of Materials Science and Engineering, Seoul National University, 599 Gwanak-ro, Gwanak-gu, Seoul 151-744, Republic of Korea
ABSTRACT There are various methods established and implemented
to prepare polymer/TiO2 nanocomposites, but the choice of preparation method is limited in the case of most frequently used commodity polymers because of their enormous production and low price. In situ suspension polymerization is rarely reported, because suspension is a severe condition to maintain the dispersion of nanoparticles in monomer phase. However, not only the incorporation of nanoparticle but also the preservation of morphology and processing condition can be attained if in situ suspension polymerization is achieved in the polymer resins mainly produced by suspension polymerization such as PVC. In this study, we prepared PVC/TiO2 nanocomposite resin via the synthesis of highly dispersible TiO2 nanoparticles in the vinyl chloride, followed by in situ suspension polymerization of vinyl chloride which contained the nanoparticles. Solvothermal method is applied to the nanoparticle preparation, and the prepared TiO2 nanoparticles have controlled sizes, shapes, and crystalline phases with the types and concentrations of precursor and oxygen donor. The film samples from prepared PVC/TiO2 nanocomposites resins are highly transparent due to the minimized visible light scattering which is an evidence of high dispersity of TiO2 nanoparticles.
Keywords: nanocomposite, titanium dioxide, poly(vinyl chloride), in situ suspension polymerization
1 INTRODUCTION Polymer/inorganic nanocomposites have been
extensively studied in the last decade. They combine the advantages of the polymer and the inorganic material, and usually contain special properties of nanofillers leading to materials with improved properties. Among the various inorganic materials, titanium dioxide (TiO2) can be widely applied to the polymeric materials for the addition of the eco-friendly characteristics such as adsorption and catalytic degradation of various contaminations, inhibition of pathogenic microorganisms, protection of ultravisible radiation, etc. Various methods, including melt extrusion of unmodified or organically modified TiO2, dispersion of organically modified TiO2 in organic solvent followed by dissolution of the matrix polymer and solvent casting, or in
situ polymerization, are established and implemented to prepare polymer/TiO2 nanocomposites. However, the choice of nanocomposite preparation method is limited in the case of most frequently used commodity polymers such as poly(vinyl chloride) (PVC), because of their enormous production and low price. Moreover, there are considerable difficulties that TiO2 nanoparticles are easily conglomerated and not simply broken apart by conventional methods. It is obvious that the most important factors which affect the properties of nanocomposites are the dispersion and the adhesion at the polymer and nanofillers . The agglomerates of TiO2 nanoparticles act as defects which inevitably result in the degradation of the mechanical properties in polymer/inorganic nanocomposites. The decrement of interface area between the polymer matrix and TiO2 due to the agglomeration, moreover, leads to inferior catalytic activity of TiO2. Therefore, it is necessary to find the preparation route which satisfies high performance-cost balance in the area of polymer/TiO2 nanocomposites.
The majority of vinyl polymers are produced by heterogeneous polymerization, e.g. emulsion polymerization, dispersion polymerization, and suspension polymerization. In situ emulsion polymerization is the most important method for polymer encapsulation of inorganic particles by far . On the other hand, in situ suspension polymerization is rarely reported, because the suspension obtained by shearing a system containing monomer, water, and suspending agent is a severe condition to maintain the dispersion of nanoparticles in monomer phase. However, not only the incorporation of nanoparticle but also the preservation of morphology and processing condition can be attained if in situ suspension polymerization is achieved in the polymer resins mainly produced by suspension polymerization such as PVC. In this study, we prepared PVC/TiO2 nanocomposite resin via the synthesis of highly dispersible TiO2 nanoparticles in the vinyl chloride (VC), the monomer of PVC, and in situ suspension polymerization of VC which contained the nanoparticles. Solvothermal method is applied to the nanoparticle preparation , and the prepared TiO2 nanoparticles have controlled sizes, shapes, and crystalline phases with the types and concentrations of precursor and oxygen donor. The sizes and shapes of the nanoparticles are determined by high-resolution transmission electron microscopy (HR- TEM), and the size distributions of the nanoparticles are determined by dynamic light scattering (DLS) method. The prepared TiO2 nanoparticles are finally incorporated in the
NSTI-Nanotech 2010, www.nsti.org, ISBN 978-1-4398-3401-5 Vol. 1, 2010740
polymer matrix through in situ suspension polymerization. The film samples from prepared PVC/TiO2 nanocomposites resins are highly transparent due to the minimized visible light scattering which is an evidence of high dispersity of TiO2 nanoparticles. The predominant dispersions of the nanoparticles are confirmed by transmission electron microscopic and UV-visible transmittance observations of prepared PVC/TiO2 nanocomposites.
Titanium tetrabutoxide (Ti(OBu)4, 98%) and titanium tetraisopropoxide (Ti(iPr)4, 98%) used in the preparation of TiO2 were obtained from Aldrich. Lauric acid, stearic acid, oleic acid, and linoleic acid used for the surface capping of TiO2 were also from Aldrich. Ethanol, cyclohexane, and tetrahydrofuran were of the highest purity available and purchased from Dae Jung Chem. All materials were used without further purification.
Reagents used for suspension polymerization were obtained from the following sources: vinyl chloride (VC) from Korea Gas; octyl peroxyneodecanoate (BND) and dioctyl peroxydicarbonate (OPP) from Chemex Co. Ltd.; poly(vinyl alcohol) (trade name K-420TM) from Kuraray Co. Ltd.; octadecyl dibutyl-4-hydroxyphenylpropionate (IR), dilauryl thiodipropionate (DL), and aluminum sulfate (AS) from Hanwha Chem. Corp. All of these chemicals were used as received.
2.2 Synthesis of TiO2 nanoparticles
In the typical synthesis procedure of TiO2 nanoparticles, Ti(OBu)4 (2 mL), lauric acid (0.05 mol), and liquefied VC (50 g) were mixed at room temperature by mechanical stirring. After continued stirring at room temperature for 10 min, the solution was kept at 80~100 °C for 6~12 h.
Before characterization of TiO2 nanoparticles, VC was slowly vented out and the residual VC was evaporated at room temperature. Organic-capped TiO2 nanoparticles were easily redispersed in solvents such as cyclohexane or tetrahydrofuran. An as-obtained sol of TiO2 nanoparticle materials could be stable for a few weeks. By adding an excess of ethanol, TiO2 nanoparticles were precipitated at room temperature. The resulting precipitates were isolated by centrifugation and washed with ethanol to remove surfactant residuals. 2.3 Preparation of poly(vinyl chloride)/TiO2 nanocomposite resin
In a high-pressure PVC polymerization reactor equipped with a temperature controller, a high-speed mechanical agitator, and a balance-controlled vacuum VC feeder, PVC/TiO2 nanocomposite resin was prepared by in-situ suspension polymerization of VC which
contained the TiO2 nanoparticles. A schematic illustration of the reaction procedure is shown in Figure 1. The experimental procedure was as follows. First, the reactor was charged with water and additives. The additives used in the suspension polymerization were K- 420TM (as a suspending agent), BND and OPP (as initiators), IR and DL (as antioxidants), and AS (as a scale inhibitor); these additives were combined in the reactor. After TiO2 nanoparticle dispersion in vinyl monomer is added to the dispersion, polymerization was carried out at a temperature of 57.5 ± 0.5 °C and a pressure of approximately 9.0 ± 0.5 bar while agitating the suspension at a speed of ca. 600 to 700 rpm until there was a pressure drop of approximately 0.5 bar from the maximum pressure attained. At the end of the reaction, the remaining gas was vented out. The crude product was then washed several times with ethanol and water, filtered, and dried overnight under vacuum.
Figure 1: Schematic illustration of the synthetic pathway for the preparation of PVC/TiO2 nanocomposite resin.
2.4 Characterization Techniques
Transmission electron microscopy (TEM). TEM images of TiO2 nanoparticles were obtained using a JEOL JEM- 3010 microscope operating at 300 kV. The samples were prepared by dropping dilute solutions of TiO2 nanoparticles in tetrahydrofuran onto 300-mesh carbon-coated copper grids and immediately evaporating the solvent. TEM images of PVC/TiO2 nanocomposite were obtained using a Philips CM20 microscope operating at 200 kV. Ultra-thin cross-sections of the specimens were prepared using a Leica Ultracut UCT ultramicrotome at room temperature.
Powder X-ray Diffraction (XRD). XRD patterns of TiO2 nanocrystal powders were collec